# CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS

Save this PDF as:

Size: px
Start display at page:

## Transcription

1 CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and Self-Interstitials 5.1 Calculate the fraction of atom sites that are vacant for copper at its melting temperature of 1084 C (1357 K). Assume an energy for vacancy formation of 0.90 ev/atom. In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation 5.1. As stated in the problem, Q v 0.90 ev/atom. Thus, N v N exp Q v 0.90 ev /atom exp kt ( ev/atom- K) (1357 K)

2 5.2 Calculate the energy for vacancy formation in silver, given that the equilibrium number of vacancies at 800 C (1073 K) is m 3. The atomic weight and density (at 800 C) for silver are, respectively, g/mol and 9.5 g/cm 3. This problem calls for the computation of the activation energy for vacancy formation in silver. Upon examination of Equation 5.1, all parameters besides Q v are given except N, the total number of atomic sites. However, N is related to the density, (ρ), Avogadro's number (N A ), and the atomic weight (A) according to Equation 5.2 as N N A ρ Pb A Pb ( atoms /mol)(9.5 g /cm 3 ) g /mol atoms/cm atoms/m 3 Now, taking natural logarithms of both sides of Equation 5.1, ln N v lnn Q v kt and, after some algebraic manipulation N Q v kt ln v N Now, inserting values for the parameters given in the problem statement leads to Q v ( m ev/atom- K)(800 C K) ln m ev/atom

3 Point Defects in Ceramics 5.3 Calculate the fraction of lattice sites that are Schottky defects for cesium chloride at its melting temperature (645 C). Assume an energy for defect formation of 1.86 ev. In order to solve this problem it is necessary to use Equation 5.4 and solve for the N s /N ratio. Rearrangement of this expression and substituting values for the several parameters leads to N s N exp Q s 2kT exp 1.86 ev (2)( ev/k)( K)

4 5.4 Using the data given below that relate to the formation of Schottky defects in some oxide ceramic (having the chemical formula MO), determine the following: (a) the energy for defect formation (in ev), (b) the equilibrium number of Schottky defects per cubic meter at 0 C, and (c) the identity of the oxide (i.e., what is the metal M?) T ( C) ρ (g/cm 3 ) N s (m 3 ) ? The (a) portion of the problem asks that we compute the energy for defect formation. To begin, let us combine a modified form of Equation 5.2 and Equation 5.4 as N s N exp Q s 2kT N A ρ A M + A exp Q s O 2kT Inasmuch as this is a hypothetical oxide material, we don't know the atomic weight of metal M, nor the value of Q s in the above equation. Therefore, let us write equations of the above form for two temperatures, T 1 and T 2. These are as follows: N s1 N A ρ 1 A M + A exp Q s O 2kT 1 (5.S1a) N s2 N A ρ 2 A M + A exp Q s O 2kT 2 (5.S1b) Dividing the first of these equations by the second leads to

5 N s1 N s2 N A ρ 1 A M + A exp Q s O 2kT 1 N A ρ 2 A M + A exp Q s O 2kT 2 which, after some algebraic manipulation, reduces to the form N s1 ρ 1 exp Q s N s2 ρ 2 2k 1 T 1 1 T 2 (5.S2) Now, taking natural logarithms of both sides of this equation gives ln N s1 N ln ρ 1 s2 ρ Q s 1 2 2k T 1 1 T 2 and solving for Q s leads to the expression Q s 2k ln N s1 N ln ρ 1 s2 ρ 2 1 T 1 1 T 2 Let us take T C and T C, and we may compute the value of Q s as Q s (2)( ev/k) ln 9 m g/cm m -3 ln 3.40 g/cm K K 7.70 ev (b) It is now possible to solve for N s at 0 C using Equation 5.S2 above. This time let's take T 1 0 C and T C. Thus, solving for N s1, substituting values provided in the problem statement and Q s determined above yields

6 N s1 N s2 ρ 1 ρ 2 exp Q s 1 2k T 1 1 T 2 ( m -3 )( 3.45 g/cm 3 ) 3.50 g/cm 3 exp 7.70 ev 1 (2)( ev/k) K K m -3 (c) And, finally, we want to determine the identity of metal M. This is possible by computing the atomic weight of M (A M ) from Equation 5.S1a. Rearrangement of this expression leads to N A ρ 1 A M + A N s1 exp Q s O 2kT 1 And, after further algebraic manipulation N A ρ 1 Q N s1 exp s 2kT 1 A M + A O And, solving this expression for A M gives A M N A ρ 1 Q N s1 exp s 2kT 1 A O Now, assuming that T C, the value of A M is A M ( ions/mol)( 3.50 g/cm 3 )(10 6 cm 3 /m 3 ) ( ions/m ev ) exp (2)( ev/k)( K) g/mol g/mol

7 Upon consultation of the periodic table in Figure 2.6, the divalent metal (i.e., that forms M 2+ ions) that has an atomic weight closest to g/mol is magnesium. Thus, this metal oxide is MgO.

8 Impurities in Solids 5.5 Below, atomic radius, crystal structure, electronegativity, and the most common valence are tabulated, for several elements; for those that are nonmetals, only atomic radii are indicated. Atomic Crystal Electro- Element Radius (nm) Structure negativity Valence Ni FCC C H O Ag FCC Al FCC Co HCP Cr BCC Fe BCC Pt FCC Zn HCP Which of these elements would you expect to form the following with nickel: (a) A substitutional solid solution having complete solubility (b) A substitutional solid solution of incomplete solubility (c) An interstitial solid solution In this problem we are asked to cite which of the elements listed form with Ni the three possible solid solution types. For complete substitutional solubility the following criteria must be met: 1) the difference in atomic radii between Ni and the other element (ΔR%) must be less than ±15%, 2) the crystal structures must be the same, 3) the electronegativities must be similar, and 4) the valences should be the same, or nearly the same. Below are tabulated, for the various elements, these criteria.

9 Crystal ΔElectro- Element ΔR% Structure negativity Valence Ni FCC 2+ C 43 H 63 O 52 Ag +16 FCC Al +15 FCC Co +0.6 HCP 0 2+ Cr +0.2 BCC Fe -0.4 BCC 0 2+ Pt +11 FCC Zn +7 HCP (a) Pt is the only element that meets all of the criteria and thus forms a substitutional solid solution having complete solubility. At elevated temperatures Co and Fe experience allotropic transformations to the FCC crystal structure, and thus display complete solid solubility at these temperatures. (b) Ag, Al, Co, Cr, Fe, and Zn form substitutional solid solutions of incomplete solubility. All these metals have either BCC or HCP crystal structures, and/or the difference between their atomic radii and that for Ni are greater than ±15%, and/or have a valence different than 2+. (c) C, H, and O form interstitial solid solutions. These elements have atomic radii that are significantly smaller than the atomic radius of Ni.

10 5.6 (a) Suppose that CaO is added as an impurity to Li 2 O. If the Ca 2+ substitutes for Li +, what kind of vacancies would you expect to form? How many of these vacancies are created for every Ca 2+ added? (b) Suppose that CaO is added as an impurity to CaCl 2. If the O 2 substitutes for Cl, what kind of vacancies would you expect to form? How many of these vacancies are created for every O 2 added? (a) For Ca 2+ substituting for Li + in Li 2 O, lithium vacancies would be created. For each Ca 2+ substituting for Li +, one positive charge is added; in order to maintain charge neutrality, a single positive charge may be removed. Positive charges are eliminated by creating lithium vacancies, and for every Ca 2+ ion added, a single lithium vacancy is formed. (b) For O 2- substituting for Cl - in CaCl 2, chlorine vacancies would be created. For each O 2- substituting for a Cl -, one negative charge is added; negative charges are eliminated by creating chlorine vacancies. In order to maintain charge neutrality, one O 2- ion will lead to the formation of one chlorine vacancy.

11 Specification of Composition 5.7 What is the composition, in atom percent, of an alloy that consists of 92.5 wt% Ag and 7.5 wt% Cu? In order to compute composition, in atom percent, of a 92.5 wt% Ag-7.5 wt% Cu alloy, we employ Equation 5.9 as C ' Ag C Ag A Cu C Ag A Cu + C Cu A Ag (92.5)(63.55 g /mol) (92.5)(63.55 g /mol) + (7.5)(107.87g /mol) 87.9 at% C ' Cu C Cu A Ag C Ag A Cu + C Cu A Ag (7.5)( g /mol) (92.5)(63.55 g /mol) + (7.5)(107.87g /mol) 12.1 at%

12 5.8 Calculate the composition, in weight percent, of an alloy that contains 105 kg of iron, 0.2 kg of carbon, and 1.0 kg of chromium. The concentration, in weight percent, of an element in an alloy may be computed using a modified form of Equation 5.6. For this alloy, the concentration of iron (C Fe ) is just C Fe m Fe m Fe + m C + m Cr 105 kg 105 kg kg kg wt% Similarly, for carbon C C 0.2 kg 105 kg kg kg 0.19 wt% And for chromium C Cr 1.0 kg 105 kg kg kg 0.94 wt%

13 5.9 What is the composition, in atom percent, of an alloy that contains 44.5 lb m of silver, 83.7 lb m of gold, and 5.3 lb m of Cu? To determine the concentrations, in atom percent, of the Ag-Au-Cu alloy, it is first necessary to convert the amounts of Ag, Au, and Cu into grams. m ' Ag (44.5 lb m )(453.6 g/lb m ) 20,185 g m ' Au (83.7 lb m )(453.6 g/lb m ) 37,966 g m ' Cu (5.3 lb m )(453.6 g/lb m ) 2, 404 g These masses must next be converted into moles (Equation 5.7), as n mag m ' Ag A Ag 20,185 g g /mol mol n mau 37,966 g g /mol mol n mcu 2, 404 g g /mol 37.8 mol Now, employment of a modified form of Equation 5.8, gives C ' Ag n mag n mag + n mau + n mcu mol mol mol mol 44.8 at% C ' Au mol mol mol mol 46.2 at%

14 C ' Cu 37.8 mol mol mol mol 9.0 at%

15 5.10 Convert the atom percent composition in Problem 5.9 to weight percent. The composition in atom percent for Problem 5.9 is 44.8 at% Ag, 46.2 at% Au, and 9.0 at% Cu. Modification of Equation 5.10 to take into account a three-component alloy leads to the following C Ag C ' Ag C ' Ag A Ag A Ag + C ' Au A Au + C ' Cu A Cu (44.8) ( g /mol) (44.8)( g /mol) + (46.2) ( g /mol) + (9.0) (63.55 g /mol) 33.3 wt% C Au C ' Ag C ' Au A Au A Ag + C ' Au A Au + C ' Cu A Cu (46.2) ( g /mol) (44.8)( g /mol) + (46.2) ( g /mol) + (9.0) (63.55 g /mol) 62.7 wt% C Cu C ' Ag C ' Cu A Cu A Ag + C ' Au A Au + C ' Cu A Cu (9.0) (63.55 g /mol) (44.8)( g /mol) + (46.2) ( g /mol) + (9.0) (63.55 g /mol) 4.0 wt%

16 5.11 Determine the approximate density of a Ti-6Al-4V titanium alloy that has a composition of 90 wt% Ti, 6 wt% Al, and 4 wt% V. In order to solve this problem, Equation 5.13a is modified to take the following form: ρ ave C Ti ρ Ti + C Al ρ Al + C V ρ V And, using the density values for Ti, Al, and V i.e., 4.51 g/cm 3, 2.71 g/cm 3, and 6.10 g/cm 3 (as taken from inside the front cover of the text), the density is computed as follows: ρ ave 90 wt% 4.51 g /cm wt% 2.71 g /cm wt% 6.10 g /cm g/cm 3

17 5.12 Some hypothetical alloy is composed of 25 wt% of metal A and 75 wt% of metal B. If the densities of metals A and B are 6.17 and 8.00 g/cm 3, respectively, whereas their respective atomic weights are and g/mol, determine whether the crystal structure for this alloy is simple cubic, face-centered cubic, or body-centered cubic. Assume a unit cell edge length of nm. In order to solve this problem it is necessary to employ Equation 3.5; in this expression density and atomic weight will be averages for the alloy that is ρ ave na ave V C N A Inasmuch as for each of the possible crystal structures, the unit cell is cubic, then V C a 3, or ρ ave na ave a 3 N A And, in order to determine the crystal structure it is necessary to solve for n, the number of atoms per unit cell. For n 1, the crystal structure is simple cubic, whereas for n values of 2 and 4, the crystal structure will be either BCC or FCC, respectively. When we solve the above expression for n the result is as follows: n ρ ave a3 N A A ave Expressions for A ave and ρ ave are found in Equations 5.14a and 5.13a, respectively, which, when incorporated into the above expression yields n C A + C a B 3 N A ρ A ρ B C A + C B A A A B

18 Substitution of the concentration values (i.e., C A 25 wt% and C B 75 wt%) as well as values for the other parameters given in the problem statement, into the above equation gives n ( wt% 6.17 g/cm wt% -8 nm) 3 ( atoms/mol) 8.00 g/cm 3 25 wt% g/mol + 75 wt% g/mol 1.00 atom/unit cell Therefore, on the basis of this value, the crystal structure is simple cubic.

19 5.13 Molybdenum forms a substitutional solid solution with tungsten. Compute the number of molybdenum atoms per cubic centimeter for a molybdenum-tungsten alloy that contains 16.4 wt% Mo and 83.6 wt% W. The densities of pure molybdenum and tungsten are and g/cm 3, respectively. To solve this problem, employment of Equation 5.21 (which derivation is called for in problem W5.16 on the book s Web site) is necessary, using the following values: C 1 C Mo 16.4 wt% ρ 1 ρ Mo g/cm 3 ρ 2 ρ W 19.3 g/cm 3 A 1 A Mo g/mol Thus N Mo C Mo A Mo ρ Mo N A C Mo + A Mo ρ W ( C Mo ) ( atoms /mol) (16.4 wt%) (16.4 wt%)(95.94 g /mol) g /mol g /cm 3 + ( 16.4 wt%) 19.3 g /cm atoms/cm 3

20 5.14 Sometimes it is desirable to be able to determine the weight percent of one element, C 1, that will produce a specified concentration in terms of the number of atoms per cubic centimeter, N 1, for an alloy composed of two types of atoms. This computation is possible using the following expression: C N A ρ 2 N 1 A 1 ρ 2 ρ 1 (5.22) where N A Avogadro s number ρ 1 and ρ 2 densities of the two elements A 1 and A 2 the atomic weights of the two elements Derive Equation 5.22 using Equation 5.2 and expressions contained in Section 5.6. The number of atoms of component 1 per cubic centimeter is just equal to the atom fraction of component 1 (c ' 1 ) times the total number of atoms per cubic centimeter in the alloy (N). Thus, using the equivalent of Equation 5.2, we may write N 1 c 1 ' N c 1 ' N A ρ ave A ave Realizing that c ' 1 C 1 ' and C 2 ' C 1 ' and substitution of the expressions for ρ ave and A ave, Equations 5.13b and 5.14b, respectively, leads to N 1 c 1 ' N A ρ ave A ave

21 N A C 1 ' ρ 1 ρ 2 C 1 ' ρ 2 A 1 + ( C 1 ' )ρ 1 A 2 And, solving for C 1 ' C 1 ' N 1 ρ 1 A 2 N A ρ 1 ρ 2 N 1 ρ 2 A 1 + N 1 ρ 1 A 2 Substitution of this expression for C ' 1 into Equation 5.10a, which may be written in the following form C 1 C 1 ' A 1 C 1 ' A 1 + C 2 ' A 2 C 1 ' A 1 C 1 ' A 1 + ( C 1 ' )A 2 yields C N A ρ 2 N 1 A 1 ρ 2 ρ 1 the desired expression.

22 5.15 Germanium forms a substitutional solid solution with silicon. Compute the weight percent of germanium that must be added to silicon to yield an alloy that contains Ge atoms per cubic centimeter. The densities of pure Ge and Si are 5.32 and 2.33 g/cm 3, respectively. To solve this problem, employment of Equation 5.22 is necessary, using the following values: N 1 N Ge 2.43 x atoms/cm 3 ρ 1 ρ Ge 5.32 g/cm 3 ρ 2 ρ Si 2.33 g/cm 3 A 1 A Ge g/mol A 2 A Si g/mol Thus C Ge 1 + N A ρ Si ρ Si N Ge A Ge ρ Ge 1 + ( atoms /mol)(2.33 g /cm 3 ) ( atoms /cm 3 ) (72.64 g /mol) 2.33 g /cm g /cm wt%

23 5.16 Iron and vanadium both have the BCC crystal structure, and V forms a substitutional solid solution for concentrations up to approximately 20 wt% V at room temperature. Compute the unit cell edge length for a 90 wt% Fe 10 wt% V alloy. First of all, the atomic radii for Fe and V (using the table inside the front cover) are and nm, respectively. Also, using Equation 3.5 it is possible to compute the unit cell volume, and inasmuch as the unit cell is cubic, the unit cell edge length is just the cube root of the volume. However, it is first necessary to calculate the density and average atomic weight of this alloy using Equations 5.13a and 5.14a. Inasmuch as the densities of iron and vanadium are 7.87g/cm 3 and 6.10 g/cm 3, respectively, (as taken from inside the front cover), the average density is just ρ ave C V + C Fe ρ V ρ Fe 10 wt% 6.10 g /cm wt% 7.87 g /cm g/cm 3 And for the average atomic weight A ave C V + C Fe A V A Fe 10 wt% g /mole + 90 wt% g /mol g/mol Now, V C is determined from Equation 3.5 as V C na ave ρ ave N A

24 (2 atoms / unit cell)(55.32 g / mol) (7.65 g /cm 3 )( atoms /mol) cm 3 /unit cell And, finally a (V C ) 1/3 ( cm 3 /unit cell) 1/ x 10-8 cm nm

25 Interfacial Defects 5.17 For an FCC single crystal, would you expect the surface energy for a () plane to be greater or less than that for a (111) plane? Why? (Note: You may want to consult the solution to Problem W3.46 at the end of Chapter 3.) The surface energy for a crystallographic plane will depend on its packing density [i.e., the planar density (Section 3.11)] that is, the higher the packing density, the greater the number of nearest-neighbor atoms, and the more atomic bonds in that plane that are satisfied, and, consequently, the lower the surface energy. From the 1 solution to Problem W3.46, planar densities for FCC () and (111) planes are 4R 2 and 1 2R 2 3, respectively that is and R 2 R 2 (where R is the atomic radius). Thus, since the planar density for (111) is greater, it will have the lower surface energy.

26 5.18 (a) For a given material, would you expect the surface energy to be greater than, the same as, or less than the grain boundary energy? Why? (b) The grain boundary energy of a small-angle grain boundary is less than for a high-angle one. Why is this so? (a) The surface energy will be greater than the grain boundary energy. For grain boundaries, some atoms on one side of a boundary will bond to atoms on the other side; such is not the case for surface atoms. Therefore, there will be fewer unsatisfied bonds along a grain boundary. (b) The small-angle grain boundary energy is lower than for a high-angle one because more atoms bond across the boundary for the small-angle, and, thus, there are fewer unsatisfied bonds.

27 5.19 For each of the following stacking sequences found in FCC metals, cite the type of planar defect that exists: (a)... A B C A B C B A C B A... (b)... A B C A B C B C A B C... Now, copy the stacking sequences and indicate the position(s) of planar defect(s) with a vertical dashed line. (a) The interfacial defect that exists for this stacking sequence is a twin boundary, which occurs at the indicated position. The stacking sequence on one side of this position is mirrored on the other side. (b) The interfacial defect that exists within this FCC stacking sequence is a stacking fault, which occurs between the two lines. Within this region, the stacking sequence is HCP.

28 Grain Size Determination 5.20 (a) Employing the intercept technique, determine the average grain size for the steel specimen whose microstructure is shown in Figure 10.29(a); use at least seven straight-line segments. (b) Estimate the ASTM grain size number for this material. (a) This portion of the problem calls for a determination of the average grain size of the specimen which microstructure is shown in Figure 10.29(a). Seven line segments were drawn across the micrograph, each of which was 60 mm long. The average number of grain boundary intersections for these lines was 6.3. Therefore, the average line length intersected is just 60 mm mm Hence, the average grain diameter, d, is d ave. line length intersected magnification 9.5 mm mm (b) This portion of the problem calls for us to estimate the ASTM grain size number for this same material. The average grain size number, n, is related to the number of grains per square inch, N, at a magnification of according to Equation However, the magnification of this micrograph is not x, but rather 90. Consequently, it is necessary to use Equation 5.20 M 2 N M 2 n 1 where N M the number of grains per square inch at magnification M, and n is the ASTM grain size number. Taking logarithms of both sides of this equation leads to the following: log N M M + 2 log (n 1) log 2 Solving this expression for n gives n M log N M + 2 log + 1 log 2

29 From Figure 10.29(a), N M is measured to be approximately 4, which leads to n log log log 2 2.7

30 5.21 For an ASTM grain size of 6, approximately how many grains would there be per square inch at (a) a magnification of, and (b) without any magnification? (a) This part of problem asks that we compute the number of grains per square inch for an ASTM grain size of 6 at a magnification of. All we need do is solve for the parameter N in Equation 5.19, inasmuch as n 6. Thus N 2 n grains/in. 2 (b) Now it is necessary to compute the value of N for no magnification. In order to solve this problem it is necessary to use Equation 5.20: M 2 N M 2 n 1 where N M the number of grains per square inch at magnification M, and n is the ASTM grain size number. Without any magnification, M in the above equation is 1, and therefore, 1 2 N And, solving for N 1, N 1 320,000 grains/in. 2.

31 of Determine the ASTM grain size number if 25 grains per square inch are measured at a magnification In order to solve this problem we make use of Equation 5.20 viz. M 2 N M 2 n 1 where N M the number of grains per square inch at magnification M, and n is the ASTM grain size number. Solving the above equation for n, and realizing that N M 25, while M 75, we have n M log N M + 2 log + 1 log 2 75 log log log

32 DESIGN PROBLEMS Specification of Composition 5.D1 Aluminum lithium alloys have been developed by the aircraft industry to reduce the weight and improve the performance of its aircraft. A commercial aircraft skin material having a density of 2.47 g/cm 3 is desired. Compute the concentration of Li (in wt%) that is required. This problem calls for us to compute the concentration of lithium (in wt%) that, when added to aluminum, will yield a density of 2.47 g/cm 3. of this problem requires the use of Equation 5.13a, which takes the form ρ ave C Li + C Li ρ Li ρ Al inasmuch as C Li + C Al. According to the table inside the front cover, the respective densities of Li and Al are and 2.71 g/cm 3. Upon solving for C Li from the above equation, we get C Li ρ Li (ρ Al ρ ave ) ρ ave (ρ Al ρ Li ) ()(0.534 g /cm3 )(2.71 g /cm g /cm 3 ) (2.47 g /cm 3 )(2.71 g /cm g /cm 3 ) 2.38 wt%

33 5.D2 Gallium arsenide (GaAs) and indium arsenide (InAs) both have the zinc blende crystal structure and are soluble in each other at all concentrations. Determine the concentration in weight percent of InAs that must be added to GaAs to yield a unit cell edge length of nm. The densities of GaAs and InAs are and g/cm 3, respectively. This problem asks that we determine the concentration (in weight percent) of InAs that must be added to GaAs to yield a unit cell edge length of nm. The densities of GaAs and InAs were given in the problem statement as and g/cm 3, respectively. To begin, it is necessary to employ Equation 3.6, and solve for the unit cell volume, V C, for the InAs-GaAs alloy as V C n' A ave ρ ave N A where A ave and ρ ave are the atomic weight and density, respectively, of the InAs-GaAs alloy. Inasmuch as both of these materials have the zinc blende crystal structure, which has cubic symmetry, V C is just the cube of the unit cell length, a. That is V C a 3 ( nm) 3 ( cm) cm 3 It is now necessary to construct expressions for A ave and ρ ave in terms of the concentration of indium arsenide, C InAs using Equations 5.14a and 5.13a. For A ave we have A ave C InAs + ( C InAs ) A InAs A GaAs C InAs g /mol + ( C InAs ) g /mol whereas for ρ ave

34 ρ ave C InAs + ( C InAs ) ρ InAs ρ GaAs C InAs g /cm 3 + ( C InAs ) g /cm 3 Within the zinc blende unit cell there are four formula units, and thus, the value of n' in Equation 3.6 is 4; hence, this expression may be written in terms of the concentration of InAs in weight percent as follows: V C x cm 3 n' A ave ρ ave N A (4 fu /unit cell) C InAs + ( C ) InAs g /mol g /mol C InAs g /cm 3 + ( C ) ( fu /mol) InAs g /cm 3 And solving this expression for C InAs leads to C InAs 46.1 wt%.

### CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS ev /atom = exp. kt ( =

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and Self-Interstitials 5.1 Calculate the fraction of atom sites that are vacant for copper at its melting temperature of 1084 C (1357 K). Assume

### Point Defects in Metals

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Point Defects in Metals 5.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 327 C (600 K). Assume an energy

### Impurities in Solids. Crystal Electro- Element R% Structure negativity Valence

4-4 Impurities in Solids 4.4 In this problem we are asked to cite which of the elements listed form with Ni the three possible solid solution types. For complete substitutional solubility the following

### 3.40 Sketch within a cubic unit cell the following planes: (a) (01 1 ) (b) (112 ) (c) (102 ) (d) (13 1) Solution

3.40 Sketch within a cubic unit cell the following planes: (a) (01 1 ) (b) (11 ) (c) (10 ) (d) (13 1) The planes called for are plotted in the cubic unit cells shown below. 3.41 Determine the Miller indices

### Density Computations

CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS Fundamental Concepts 3.1 What is the difference between atomic structure and crystal structure? Unit Cells Metallic Crystal Structures 3.2 If the atomic radius

### Structure of silica glasses (Chapter 12)

Questions and Problems 97 Glass Ceramics (Structure) heat-treated so as to become crystalline in nature. The following concept map notes this relationship: Structure of noncrystalline solids (Chapter 3)

### Fundamental concepts and language Unit cells Crystal structures! Face-centered cubic! Body-centered cubic! Hexagonal close-packed Close packed

Fundamental concepts and language Unit cells Crystal structures! Face-centered cubic! Body-centered cubic! Hexagonal close-packed Close packed crystal structures Density computations Crystal structure

### Chapter Outline. How do atoms arrange themselves to form solids?

Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures! Face-centered cubic! Body-centered cubic! Hexagonal close-packed Close packed

### Chapter Outline How do atoms arrange themselves to form solids?

Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Face-centered cubic Body-centered cubic Hexagonal close-packed Close packed

### Materials and their structures

Materials and their structures 2.1 Introduction: The ability of materials to undergo forming by different techniques is dependent on their structure and properties. Behavior of materials depends on their

### CRYSTAL STRUCTURE, MECHANICAL BEHAVIOUR & FAILURE OF MATERIALS

MODULE ONE CRYSTAL STRUCTURE, MECHANICAL BEHAVIOUR & FAILURE OF MATERIALS CRYSTAL STRUCTURE Metallic crystal structures; BCC, FCC and HCP Coordination number and Atomic Packing Factor (APF) Crystal imperfections:

### CHAPTER 10 PHASE DIAGRAMS PROBLEM SOLUTIONS

CHAPTER 10 PHASE DIAGRAMS PROBLEM SOLUTIONS Solubility Limit 10.1 Consider the sugar water phase diagram of Figure 10.1. (a) How much sugar will dissolve in 1000 g of water at 80 C (176 F)? (b) If the

### CHAPTER 3: CRYSTAL STRUCTURES & PROPERTIES

CHAPTER 3: CRYSTAL STRUCTURES & PROPERTIES ISSUES TO ADDRESS... How do atoms assemble into solid structures? (for now, focus on metals) How does the density of a material depend on its structure? When

### Packing of atoms in solids

MME131: Lecture 6 Packing of atoms in solids A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s topics Atomic arrangements in solids Points, directions and planes in unit cell References:

### Energy and Packing. Materials and Packing

Energy and Packing Non dense, random packing Energy typical neighbor bond length typical neighbor bond energy r Dense, regular packing Energy typical neighbor bond length typical neighbor bond energy r

### HOMEWORK 6. solutions

HOMEWORK 6. SCI 1410: materials science & solid state chemistry solutions Textbook Problems: Imperfections in Solids 1. Askeland 4-67. Why is most gold or siler jewelry made out of gold or siler alloyed

### TOPIC 2. STRUCTURE OF MATERIALS III

Universidad Carlos III de Madrid www.uc3m.es MATERIALS SCIENCE AND ENGINEERING TOPIC 2. STRUCTURE OF MATERIALS III Topic 2.3: Crystalline defects. Solid solutions. 1 PERFECT AND IMPERFECT CRYSTALS Perfect

### Introduction to Materials Science and Engineering

01 Askeland Chap 9/27/05 1:48 PM Page 1 1 Introduction to Materials Science and Engineering 1 4 Steel is often coated with a thin layer of zinc if it is to be used outside. What characteristics do you

### Defects and Diffusion

Defects and Diffusion Goals for the Unit Recognize various imperfections in crystals Point imperfections Impurities Line, surface and bulk imperfections Define various diffusion mechanisms Identify factors

### Introduction to the phase diagram Uses and limitations of phase diagrams Classification of phase diagrams Construction of phase diagrams

Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka Concept of alloying Classification of alloys Introduction to the phase diagram Uses and limitations of phase diagrams Classification of phase diagrams

### Chapter 3 Structure of Crystalline Solids

Chapter 3 Structure of Crystalline Solids Crystal Structures Points, Directions, and Planes Linear and Planar Densities X-ray Diffraction How do atoms assemble into solid structures? (for now, focus on

### Imperfections: Good or Bad? Structural imperfections (defects) Compositional imperfections (impurities)

Imperfections: Good or Bad? Structural imperfections (defects) Compositional imperfections (impurities) 1 Structural Imperfections A perfect crystal has the lowest internal energy E Above absolute zero

### These metal centres interact through metallic bonding

The structures of simple solids The majority of inorganic compounds exist as solids and comprise ordered arrays of atoms, ions, or molecules. Some of the simplest solids are the metals, the structures

### 7.3 Bonding in Metals > Chapter 7 Ionic and Metallic Bonding. 7.3 Bonding in Metals. 7.1 Ions 7.2 Ionic Bonds and Ionic Compounds

Chapter 7 Ionic and Metallic Bonding 7.1 Ions 7.2 Ionic Bonds and Ionic Compounds 7.3 Bonding in Metals 1 Copyright Pearson Education, Inc., or its affiliates. All Rights Reserved. CHEMISTRY & YOU What

### Point Defects. Vacancies are the most important form. Vacancies Self-interstitials

Grain Boundaries 1 Point Defects 2 Point Defects A Point Defect is a crystalline defect associated with one or, at most, several atomic sites. These are defects at a single atom position. Vacancies Self-interstitials

### Free Electron Model What kind of interactions hold metal atoms together? How does this explain high electrical and thermal conductivity?

Electrical Good conductors of heat & electricity Create semiconductors Oxides are basic ionic solids Aqueous cations (positive charge, Lewis acids) Reactivity increases downwards in family Mechanical Lustrous

### ENGINEERING MATERIALS LECTURE #4

ENGINEERING MATERIALS LECTURE #4 Chapter 3: The Structure of Crystalline Solids Topics to Cover What is the difference in atomic arrangement between crystalline and noncrystalline solids? What features

### Engineering 45: Properties of Materials Final Exam May 9, 2012 Name: Student ID number:

Engineering 45: Properties of Materials Final Exam May 9, 2012 Name: Student ID number: Instructions: Answer all questions and show your work. You will not receive partial credit unless you show your work.

### Unit-1 THE SOLID STATE QUESTIONS VSA QUESTIONS (1 - MARK QUESTIONS)

Unit-1 THE SOLID STATE QUESTIONS VSA QUESTIONS (1 - MARK QUESTIONS) 1. What are anistropic substances. 2. Why are amorphous solids isotropic in nature?. Why glass is regarded as an amorphous solid? 4.

### CHAPTER 5: DIFFUSION IN SOLIDS

CHAPTER 5: DIFFUSION IN SOLIDS ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases? How does diffusion

### Free Electron Model What kind of interactions hold metal atoms together? How does this explain high electrical and thermal conductivity?

Electrical Good conductors of heat & electricity Create semiconductors Oxides are basic ionic solids Aqueous cations (positive charge, Lewis acids) Reactivity increases downwards in family Free Electron

### Two marks questions and answers. 1. what is a Crystal? (or) What are crystalline materials? Give examples

UNIT V CRYSTAL PHYSICS PART-A Two marks questions and answers 1. what is a Crystal? (or) What are crystalline materials? Give examples Crystalline solids (or) Crystals are those in which the constituent

### Learning Objectives. Chapter Outline. Solidification of Metals. Solidification of Metals

Learning Objectives Study the principles of solidification as they apply to pure metals. Examine the mechanisms by which solidification occurs. - Chapter Outline Importance of Solidification Nucleation

### Stacking Oranges. Packing atoms together Long Range Order. What controls the nearest number of atoms? Hard Sphere Model. Hard Sphere Model.

{ Stacking atoms together Crystal Structure Stacking Oranges Packing atoms together Long Range Order Crystalline materials... atoms pack in periodic, 3D arrays typical of: -metals -many ceramics -some

### Metallic crystal structures The atomic bonding is metallic and thus non-directional in nature

Chapter 3 The structure of crystalline solids Hw: 4, 6, 10, 14, 18, 21, 26, 31, 35, 39, 42, 43, 46, 48, 49, 51, 56, 61 Due Wensday 14/10/2009 Quiz1 on Wensday 14/10/2009 Why study the structure of crystalline

### CHAPTER 9 PHASE DIAGRAMS

CHAPTER 9 PHASE DIAGRAMS PROBLEM SOLUTIONS 9.14 Determine the relative amounts (in terms of mass fractions) of the phases for the alloys and temperatures given in Problem 9.8. 9.8. This problem asks that

### (C) Na 2. (B) NaWO 3 WO 3

EXERCISE-01 CHECK YOUR GRASP SELECT THE CORRECT ALTERNATIVE (ONLY ONE CORRECT ANSWER) 1. A solid has a structure in which W atoms are located at the corners of a cubic lattice, O atom at the centre of

### CH445/545 Winter 2008

CH445/545 Winter 2008 Assignment # 1 - due 01/18/08 60 total points SHOW ALL WORKING FOR FULL CREDIT, ANSWERS WITHOUT WORKING WILL BE PENALIZED! 1. Text Ch. 1 # 2 "Calculate the size of the largest sphere

### 9/16/ :30 PM. Chapter 3. The structure of crystalline solids. Mohammad Suliman Abuhaiba, Ph.D., PE

Chapter 3 The structure of crystalline solids 1 Mohammad Suliman Abuhaiba, Ph.D., PE 2 Home Work Assignments HW 1 2, 7, 12, 17, 22, 29, 34, 39, 44, 48, 53, 58, 63 Due Sunday 17/9/2015 3 Why study the structure

### CHAPTER 2. Structural Issues of Semiconductors

CHAPTER 2 Structural Issues of Semiconductors OUTLINE 1.0 Energy & Packing 2.0 Materials & Packing 3.0 Crystal Structures 4.0 Theoretical Density, r 5.0.Polymorphism and Allotropy 6.0 Close - Packed Crystal

### Phase Transformations in Metals Tuesday, December 24, 2013 Dr. Mohammad Suliman Abuhaiba, PE 1

Ferrite - BCC Martensite - BCT Fe 3 C (cementite)- orthorhombic Austenite - FCC Chapter 10 Phase Transformations in Metals Tuesday, December 24, 2013 Dr. Mohammad Suliman Abuhaiba, PE 1 Why do we study

### ENERGY AND PACKING. Chapter 3 CRYSTAL STRUCTURE & PROPERTIES MATERIALS AND PACKING METALLIC CRYSTALS ISSUES TO ADDRESS...

Chapter 3 CRYSTAL STRUCTURE & PROPERTIES ISSUES TO ADDRESS... 1. How do s assemble into solid structures? (For now, focus on metals) ENERGY AND PACKING non dense, random packing bond energy Energy bond

### Chapter 12: Structures & Properties of Ceramics

Chapter 12: Structures & Properties of Ceramics ISSUES TO ADDRESS... Review of structures for ceramics How are impurities accommodated in the ceramic lattice? In what ways are ceramic phase diagrams similar

### Unit 1 The Solid State

Points to Remember Amorphous and Crystalline Solids Unit 1 The Solid State Amorphous- short range order, Irregular shape eg-glass Crystalline Solids- long range order, regular shape eg : NaCl Molecular

### Diffusion in Solids. Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases?

Diffusion in Solids ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases? How does diffusion depend

### Introduction to Engineering Materials ENGR2000 Chapter 3: The Structure of Crystalline Solids. Dr. Coates

Introduction to Engineering Materials ENGR2000 Chapter 3: The Structure of Crystalline Solids Dr. Coates Learning Objectives I 1. Describe difference in atomic/molecular structure between crystalline/noncrystalline

### 9/28/2013 9:26 PM. Chapter 3. The structure of crystalline solids. Dr. Mohammad Abuhaiba, PE

Chapter 3 The structure of crystalline solids 1 2 Why study the structure of crystalline solids? Properties of some materials are directly related to their crystal structure. Significant property differences

### Material Evaporation Application Comment MP P / Optical films, Oxide films, Electrical contacts. Doping, Electrical contacts.

for vapour Aluminum (Al) -, Optical, Oxide, Electrical BN liners with lid are recommended due to the reactivity and the fact that Al creeps out. Cooling down of the cell with 1K per minute. 660 972 Antimony

### 1. Use the Ellingham Diagram (reproduced here as Figure 0.1) to answer the following.

315 Problems 1. Use the Ellingham Diagram (reproduced here as Figure 0.1) to answer the following. (a) Find the temperature and partial pressure of O 2 where Ni(s), Ni(l), and NiO(s) are in equilibrium.

### 1.10 Close packed structures cubic and hexagonal close packing

1.9 Description of crystal structures The most common way for describing crystal structure is to refer the structure to the unit cell. The structure is given by the size and shape of the cell and the position

### Module-6. Dislocations and Strengthening Mechanisms

Module-6 Dislocations and Strengthening Mechanisms Contents 1) Dislocations & Plastic deformation and Mechanisms of plastic deformation in metals 2) Strengthening mechanisms in metals 3) Recovery, Recrystallization

### CHAPTER 3. Crystal Structures and Crystal Geometry 3-1

CHAPTER 3 Crystal Structures and Crystal Geometry 3-1 The Space Lattice and Unit Cells 3-2 Atoms, arranged in repetitive 3-Dimensional pattern, in long range order (LRO) give rise to crystal structure.

### Ph.D. Admission 20XX-XX Semester X

Ph.D. Admission 20XX-XX Semester X Written Examination Materials Science & Engineering Department, IIT Kanpur Date of Examination: XX XXXX 20XX Timing: XX:XX XX:XX XX Application# Please read these instructions

### REVISED PAGES IMPORTANT TERMS AND CONCEPTS REFERENCES QUESTIONS AND PROBLEMS. 166 Chapter 6 / Mechanical Properties of Metals

1496T_c06_131-173 11/16/05 17:06 Page 166 166 Chapter 6 / Mechanical Properties of Metals IMPORTANT TERMS AND CONCEPTS Anelasticity Design stress Ductility Elastic deformation Elastic recovery Engineering

### Chapter 5: Diffusion

Chapter 5: Diffusion ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases? How does diffusion depend

### Crystal Structures of Interest

rystal Structures of Interest Elemental solids: Face-centered cubic (fcc) Hexagonal close-packed (hcp) ody-centered cubic (bcc) Diamond cubic (dc) inary compounds Fcc-based (u 3 u,nal, ß-ZnS) Hcp-based

### STRENGTHENING MECHANISM IN METALS

Background Knowledge Yield Strength STRENGTHENING MECHANISM IN METALS Metals yield when dislocations start to move (slip). Yield means permanently change shape. Slip Systems Slip plane: the plane on which

### Alloys and Solid Solutions

Alloys and Solid Solutions Chemistry 123 Spring 2008 Dr. Woodward Solutions Solid Solution 14 Carat Gold Liquid Solution Vodka Gaseous Solution Air Solution = A homogeneous mixture 1 Alloys An alloy is

### A.M. MONDAY, 18 January minutes

Candidate Name Centre Number Candidate Number 0 GCSE 240/02 ADDITIONAL SCIENCE IGER TIER CEMISTRY 2 A.M. MONDAY, 18 January 2010 45 minutes ADDITIONAL MATERIALS In addition to this paper you may require

### Chapter 3: Structures of Metals & Ceramics

Chapter 3: Structures of Metals & Ceramics School of Mechanical Engineering Professor Choi, Hae-Jin Chapter 3-1 Chapter 3: Structures of Metals & Ceramics ISSUES TO ADDRESS... How do atoms assemble into

### Lecture # 11 References:

Lecture # 11 - Line defects (1-D) / Dislocations - Planer defects (2D) - Volume Defects - Burgers vector - Slip - Slip Systems in FCC crystals - Slip systems in HCP - Slip systems in BCC Dr.Haydar Al-Ethari

### J = D C A C B x A x B + D C A C. = x A kg /m 2

1. (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. (a) With vacancy diffusion, atomic

### Alloys GENERAL CONSIDERATIONS 621 SUBSTITUTIONAL SOLID SOLUTIONS HUME-ROTHERY RULES 624

ch22.qxd 9/22/4 5:29 PM Page 619 22 Alloys GENERAL CONSIDERATIONS 621 SUBSTITUTIONAL SOLID SOLUTIONS HUME-ROTHERY RULES 624 ORDER-DISORDER TRANSFORMATION 627 Elementary theory of order 629 PHASE DIAGRAMS

### Phase Diagrams of Pure Substances Predicts the stable phase as a function of P total and T. Example: water can exist in solid, liquid and vapor

PHASE DIAGRAMS Phase a chemically and structurally homogenous region of a material. Region of uniform physical and chemical characteristics. Phase boundaries separate two distinct phases. A single phase

### Chapter Outline Dislocations and Strengthening Mechanisms. Introduction

Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip

### SUB-Programs - Calibration range Fe Base for "PMI-MASTER Pro" Spark - mode Fe 000

SUB-Programs - Calibration range Fe Base for "PMI-MASTER Pro" Spark - mode Fe 100 Fe 200 *** Fe 250 *** Fe 300 Fe 400 Fe 500 Fe 000 Fe low alloy steel cast iron Cr hard / Ni resist stainless steel tool

### The structures of pure metals are crystalline (crystal lattice) with regular arrangement of metal atoms that are identical perfect spheres.

HW#3 Louisiana Tech University, Chemistry 481. POGIL (Process Oriented Guided Inquiry Learning) Exercise on Chapter 3. Metals and Alloys. Why? Metals What is the structure of a metallic solid? What is

### Chapter 10: Phase Diagrams

hapter 10: Phase Diagrams Show figures 10-1 and 10-3, and discuss the difference between a component and a phase. A component is a distinct chemical entity, such as u, Ni, NiO or MgO. A phase is a chemically

Defects in solids http://www.bath.ac.uk/podcast/powerpoint/inaugural_lecture_250407.pdf http://www.materials.ac.uk/elearning/matter/crystallography/indexingdirectionsandplanes/indexing-of-hexagonal-systems.html

### How to Make Micro/Nano Devices?

How to Make Micro/Nano Devices? Science: Physics, Chemistry, Biology, nano/biotech Materials: inorganic, organic, biological, rigid/flexible Fabrication: photo/e-beam lithography, self-assembly, D/3D print

### Point Defects LATTICE VACANCIES 585. DIFFUSION 588 Metals 591. COLOR CENTERS 592 F centers 592 Other centers in alkali halides 593 PROBLEMS 595

ch20.qxd 9/22/04 5:27 PM Page 583 20 Point Defects LATTICE VACANCIES 585 DIFFUSION 588 Metals 591 COLOR CENTERS 592 F centers 592 Other centers in alkali halides 593 PROBLEMS 595 1. Frenkel defects 595

### PROF. DR. M.M. B. EL SABBAH AL-AZHAR UNIVERSITY FACULTY OF SCIENCE CHEMISTRY DEPARTMENT

PROF. DR. M.M. B. EL SABBAH AL-AZHAR UNIVERSITY FACULTY OF SCIENCE CHEMISTRY DEPARTMENT 2016 PRINCIPLES OF CORROSION ELECTROCHEMICAL AND THERMODYNAMIC PRINCIPLES OF CORROSION Content 1. Definition of corrosion.

### LN Introduction to Solid State Chemistry. Lecture Notes No. 9 DIFFUSION

3.091 Introduction to Solid State Chemistry Lecture Notes No. 9 DIFFUSION * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * Sources for Further Reading:

### Chapter 18: Electrical Properties

Chapter 18: Electrical Properties ISSUES TO ADDRESS... How are electrical conductance and resistance characterized? What are the physical phenomena that distinguish conductors, semiconductors, and insulators?

### Chem 253, UC, Berkeley. Chem 253, UC, Berkeley

1 2 Theorem: For any family of lattice planes separated by distance d, there are reciprocal lattice vectors perpendicular to the planes, the shortest being 2 /d. Orientation of plane is determined by a

### Cu/Ag Eutectic System

Eutectic Systems The simplest kind of system with two solid phases is called a eutectic system. A eutectic system contains two solid phases at low temperature. These phases may have different crystal structures,

### Carbon nanostructures. (http://www.mf.mpg.de/de/abteilungen/schuetz/index.php?lang=en&content=researchtopics&type=specific&name=h2storage)

Carbon nanostructures (http://www.mf.mpg.de/de/abteilungen/schuetz/index.php?lang=en&content=researchtopics&type=specific&name=h2storage) 1 Crystal Structures Crystalline Material: atoms arrange into a

### Part 1. Preparation and Color of Solutions. Experiment 1 (2 session lab) Electrons and Solution Color. Pre-lab Report, page 29

Experiment 1 (2 session lab) Electrons and Solution Color Pre-lab Report, page 29 Session 1 One hour discussion (E2) Two hour lab (E1) Aim to complete Parts 1, 2, and 3 of E1. Part 1. Preparation and Color

### Review key concepts from last lecture (lattice + basis = unit cell) Bravais lattices Important crystal structures Intro to miller indices

Outline: Review key concepts from last lecture (lattice + basis = unit cell) Bravais lattices Important crystal structures Intro to miller indices Review (example with square lattice) Lattice: square,

### C h a p t e r 4 : D e f e c t s i n C r y s t a l s

C h a p t e r 4 : D e f e c t s i n C r y s t a l s...perfection's a gift of The gods, few can boast they possess it - and most Of you, my dears, don't. - Ovid, The Art of Love Chapter 4: Defects in Crystals...

### Chapter: The d and f Block Elements

Chapter: The d and f Block Elements Introduction to d block elements Question 1 In Tc ( Z = 43) and Tb( Z = 65) which one is inner transition metal and which one is transition metal and why? The outer

### Donald Neamen 물리전자 / 김삼동 1-1

An Introduction to Semiconductor Devices Donald Neamen Images and illustrations from supplements of An Introduction to Semiconductor Devices, 4 th Ed., Mc Graw Hill were used for this lecture materials.

### Chem 241. Lecture 19. UMass Amherst Biochemistry... Teaching Initiative

Chem 241 Lecture 19 UMass Amherst Biochemistry... Teaching Initiative Announcement March 26 Second Exam Recap Water Redox Comp/Disproportionation Latimer Diagram Frost Diagram Pourbaix Diagram... 2 Ellingham

### SECOND MIDTERM EXAM Chemistry April 2011 Professor Buhro

SECOND MIDTERM EXAM Chemistry 465 1 April 011 Professor Buhro Signature Print Name Clearly ID Number: Information. This is a closed-book exam; no books, notes, other students, other student exams, or any

### but T m (Sn0.62Pb0.38) = 183 C, so this is a common soldering alloy.

T m (Sn) = 232 C, T m (Pb) = 327 C but T m (Sn0.62Pb0.38) = 183 C, so this is a common soldering alloy. T m (Au) = 1064 C, T m (Si) = 2550 C but T m (Au0.97Si0.03) = 363 C, so thin layer of gold is used

### A.M. MONDAY, 18 January minutes

Candidate Name Centre Number Candidate Number 0 GCSE 240/01 ADDITIONAL SCIENCE FOUNDATION TIER CHEMISTRY 2 A.M. MONDAY, 18 January 2010 45 minutes ADDITIONAL MATERIALS In addition to this paper you may

### Basic Solid State Chemistry, 2 nd ed. West, A. R.

Basic Solid State Chemistry, 2 nd ed. West, A. R. Chapter 1 Crystal Structures Many of the properties and applications of crystalline inorganic materials revolve around a small number of structure types

### Mohammad Anwar Karim Id :

Department of Mechanical and Industrial Engineering ME 8109 Casting and Solidification of Materials EFFECTS OF RAPID SOLIDIFICATION ON MICROSTRUCTURE AND PROPERTIES OF AL, MG & TI ALLOYS Winter 2012 Presented

### Chapter 1.6. Polished Single-Crystal Silicon, Prime Wafers (all numbers nominal) Wafer Specification Table. Diameter 100 mm 4-inch 150 mm 6-inch

Chapter 1.6 I - Substrate Specifications Polished Single-Crystal Silicon, Prime Wafers (all numbers nominal) Wafer Specification Table Diameter 100 mm 4-inch 150 mm 6-inch Thickness 525 µm 20.5 mils 675

### CRYSTAL LATTICE. Defining lattice: Mathematical construct; ideally infinite arrangement of points in space.

CRYSTAL LATTICE How to form a crystal? 1. Define the structure of the lattice 2. Define the lattice constant 3. Define the basis Defining lattice: Mathematical construct; ideally infinite arrangement of

### Alloys & Their Phase Diagrams. مرجع علمى مهندسى مواد

Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Gibbs phase rule

### Teach Yourself: Phase Diagrams and Phase Transformations

Teach Yourself: Phase Diagrams and Phase Transformations Hugh Shercliff and Mike Ashby 5 th Edition, March 2009, Cambridge This Booklet is also found in Materials: Engineering, Science, Processing and

### Sputtering Targets for Microelectronics. Sputtering Targets for Semiconductor Applications

Sputtering Targets for Microelectronics Sputtering Targets for Semiconductor Applications Umicore Thin Film Products Umicore Thin Film Products, a globally active business unit within the Umicore Group,

### UNIT V -CRYSTAL STRUCTURE

UNIT V -CRYSTAL STRUCTURE Solids are of two types: Amorphous and crystalline. In amorphous solids, there is no order in the arrangement of their constituent atoms (molecules). Hence no definite structure

### Schedule of Accreditation issued by United Kingdom Accreditation Service 2 Pine Trees, Chertsey Lane, Staines-upon-Thames, TW18 3HR, UK

2 Pine Trees, Chertsey Lane, Staines-upon-Thames, TW18 3HR, UK Metals and Minerals Division 2 Perry Road Witham Essex CM8 3TU Contact: Mrs C Hargreaves Tel: +44 (0)1376 536800 Fax: +44 (0)1376 520819 E-Mail:

### 3. Anisotropic blurring by dislocations

Dynamical Simulation of EBSD Patterns of Imperfect Crystals 1 G. Nolze 1, A. Winkelmann 2 1 Federal Institute for Materials Research and Testing (BAM), Berlin, Germany 2 Max-Planck- Institute of Microstructure

### New GCSE 4462/02 SCIENCE A HIGHER TIER CHEMISTRY 1

Surname Other Names Centre Number 0 Candidate Number New GCSE 4462/02 SCIENCE A HIGHER TIER CHEMISTRY 1 ADDITIONAL MATERIALS A.M. WEDNESDAY, 18 January 2012 1 hour In addition to this paper you may require

### A DISLOCATION MODEL FOR THE PLASTIC DEFORMATION OF FCC METALS AN ANALYSIS OF PURE COPPER AND AUSTENITIC STEEL

A DISLOCATION MODEL FOR THE PLASTIC DEFORMATION OF FCC METALS AN ANALYSIS OF PURE COPPER AND AUSTENITIC STEEL Background In the bcc model for work hardening in single phase materials, see (6), it is assumed